 Nano Express
 Open Access
 Published:
Origin of the blueshift of photoluminescence in a typeII heterostructure
Nanoscale Research Letters volume 7, Article number: 654 (2012)
Abstract
Blueshifts of luminescence observed in typeII heterostructures are quantitatively examined in terms of a selfconsistent approach including excitonic effects. This analysis shows that the main contribution to the blueshift originates from the well region rather than the variation of triangular potentials formed in the barrier region. The power law for the blueshift, ΔE_{ PL } ∝ P_{ laser }^{m}, from m = 1/2 for lower excitation P_{laser} to m = 1/4 for higher excitation, is obtained from the calculated results combined with a rate equation analysis, which also covers the previously believed m = 1/3 power law within a limited excitation range. The present power law is consistent with the blueshift observed in a GaAsSb/GaAs quantum well.
Background
Interest has recently been increasing in typeII heterostructures in which electrons and holes are separated in adjacent different materials, thereby forming spatially indirect excitons [1–9]. The wavefunction of the indirect exciton is significantly extended in space compared with that of a direct exciton in a typeI system where both electrons and holes are confined in the same layer, which allows large controllability of the wavefunction distribution. In addition, the long radiative lifetime originating from spatially indirect recombination is attractive for applications such as optical memories [10, 11].
The separation of charge carriers in a typeII system also induces electrostatic potential (Hartree potential), which causes band bending and a resultant significant change in the exciton wavefunction distribution. Experimentally, this bandbending effect has been observed in powerdependent photoluminescence (PL) measurements, in the blueshift of PL peaks with increasing excitation power [1, 2, 5, 6, 12]. The mechanism of this effect has been discussed in terms of a triangular potential model in which photogenerated electrons and holes form a dipole layer, creating a triangularlike potential at the interface [1]. With increasing excitation power, the potential becomes steeper and the quantization energy increases, giving rise to a blueshift of the recombination energy. Following this model, the blueshift is proportional to the cube root of the excitation power, which has been generally accepted for the characterization and distinction of typeII heterostructures.
However, detailed examinations of the observed power dependency sometimes show deviations from the cube root of power law. This is especially noticeable when the excitation power dependence is examined over a wide range. Here, we reexamine the characteristic blueshift in a typeII system using a GaAsSb/GaAs quantum well (QW). We observe that the blueshift does not obey a singleexponent power law, but instead tends to saturate with increasing excitation power. This is analyzed on the basis of a selfconsistent band calculation. The dominant contribution to the blueshift originates from the variation of the QW energy level rather than the variation of the triangular potentials formed in the barrier layers, which modifies the cuberoot power law.
Methods
The sample containing a 6nm GaAsSb QW was grown on a GaAs(001) substrate by MOMBE. The Sb composition of GaAsSb was set at 8%, which was confirmed by XRD. At this Sb concentration, the band lineup between GaAs and GaAsSb becomes a typeII alignment with holes confined in the GaAsSb well [13, 14]. The excitation power dependence of the PL was measured at 23 K using the 633 nm line of a HeNe laser with an intensity range of 1 to 100 W cm^{2}. The incident beam was chopped using an optical chopper to avoid heating.
Results and discussion
Figure 1 shows the normalized PL spectra of the sample as a function of excitation power. The spectra show a typical blueshift with increasing excitation power. The shift of the PL peak energy is summarized in the inset, which clearly shows that the cuberoot power law only holds within a limited range. The power exponent is greater than 1/3 at low excitation, then decreases and becomes smaller than 1/3 at high excitation.
To elucidate the origin of the characteristic blueshift, let us start with a semiquantitative analysis of the band bending in a typeII system. We will deal with a single QW structure, and study the band bending effect numerically using a simple oneband model for both the electron and the heavy hole. The excitonic effect is not taken into account at this stage. The oneparticle effective mass Schrödinger equations are given by
where i = e (electron) or h (hole), m_{ iz } is the carrier effective mass in the growth direction z, V_{ i }(z) the heterostructure potential and φ(z) the selfconsistent Hartree potential induced by the spatial separation of the charged carriers. The Hartree potential is obtained from Poisson’s equation,
in which ε is the dielectric constant, ε_{0} is the permittivity of vacuum, and n_{ i } is the carrier density determined by the normalized wavefunctions ψ_{ i }(z):
The sheet charge density n_{s} is a parameter which is an increasing function of the excitation power. Equations 1, 2 and 3 are solved iteratively until they converge.
Figure 2a shows the calculated band diagram of the GaAsSb/GaAs QW for a sheet charge density n_{s} = 1 × 10^{11} cm^{2}. The selfconsistent potential is shown by the solid lines, and the flatband potential by the dashed lines. Electron and heavyhole wavefunctions with their eigenenergies under the bending band are also plotted in Figure 2a. The parameters used in the calculation are summarized in Table 1. In this heterostructure, holes are confined in the GaAsSb well, whereas electrons are loosely bound to the triangular potential wells formed at the GaAsSb/GaAs interfaces. The ground state energy of the electron under the bending band is lower than that under the flat band because of the attractive Hartree potential, which results in a redshift of the transition energy. However, the hole ground state is also pushed down by the band bending, which leads to a blueshift. The total transition energy is thus dependent on two competing shifts.
To see how the transition energy shifts with the excitation, we calculated the energy shifts of the electron and heavy hole as a function of the sheet charge density Figure 2b. The energy shift of the optical transition, ΔE_{PL}, is given by the difference between the two energy shifts: ΔE_{PL} = ΔE_{e}  ΔE_{hh}. As the sheet charge density increases, both the electron and heavyhole energy levels monotonically decrease due to the increasing Hartree potential. Furthermore, the heavyhole energy shift is always larger than the electron energy shift. As a result, the transition energy shift ΔE_{PL} shows a blueshift with increasing excitation. Indeed, this trend is generally true for a typeII structure; the confined carrier (here the hole) is more susceptible to the Hartree potential. This response is partly because the potential well for the electrons is formed at the skirt of the Hartree potential, while holes are affected by the peak height of the Hartree potential. In addition, an increase in the steepness of the triangular well for the electrons raises the quantization energy, compensating for the energy decrease due to the increased well depth.
Having confirmed that the blueshift is mainly caused by the energy shift of the hole in the well, we consider the power dependency of the peak shift. To the zeroorder approximation, the hole energy change is proportional to the depth of the Hartree potential, which is, in turn, proportional to the sheet charge density if the holes and electrons are completely separated. The calculated energy shift in Figure 2b shows sublinear dependence on the sheet charge density, indicating that the distribution of electrons and holes under the bending band plays an important role. For more quantitative evaluation, especially at low excitation regimes, it is necessary to include excitonic effects in the calculation. We performed a calculation of the exciton energy under the bending band following [17]. The Schrödinger equation for the exciton is
Here, 1/m_{ ρ } = 1/m_{ eρ } + 1/m_{ hρ } and is the inplane reduced mass, and ρ is the inplane electron–hole distance. The Hartree potential is included in the calculation through the modified heterostructure potential {\stackrel{\sim}{V}}_{i}\left({z}_{i}\right)={V}_{i}(z)\mp \varphi \left({z}_{i}\right), where i = e (electron) corresponds to the upper sign, and h (hole) to the lower sign. For simplicity, we ignore the spatially dependent dielectric screening in Equation 4. To solve Poisson’s equation, the carrier density n_{i} is obtained by
Again, the sheet charge density n_{s} is a parameter.
Figure 3a plots the probability density of the electron under the flat band (n_{s} = 0 cm^{2}) and the bending band (n_{s} = 5 × 10^{11} cm^{2}). The electron probability density is calculated from the wavefunction ψ(ρ, z_{ e }, z_{ h }) by p_{ e }(z_{ e }) = ∫ _{0}^{∞}dρ ∫ _{− ∞}^{∞}dz_{ h }2πρψ(ρ, z_{ e }, z_{ h })^{2}. It is clearly seen that the electron is attracted to the well under the flat band due to the presence of Coulomb interaction. Binding energy of 3.7 meV is obtained for the exciton by comparing with the energies of the singleparticle calculation Equation 1. Figure 3b shows the exciton energy shift in the GaAsSb/GaAs QW as a function of the sheet charge density. The energy shift increases linearly with the sheet charge density at the low density level, and subsequently shows sublinear dependence at the higher density regime. The power exponent at the high density regime is found to be approximately ~0.5. Although we do not have a clear explanation of the origin of the 1/2 exponent at the high power regime, the sublinear increase in the energy shift can be qualitatively understood in terms of the spatial distribution of the electron wavefunction. At a low charge density where the Hartree potential is small, most of the electrons remain in the GaAs barrier, and the electron probability density inside the GaAsSb well is negligibly small. Thus, the spatially separated charges increase in proportion to the sheet charge density, which results in a linear increase in the Hartree potential. In contrast, a significant portion of the electron wavefunction penetrates into the well at high charge density n_{s} = 5 × 10^{11} cm^{2}. This penetration decreases the net charge that forms the Hartree potential, leading to the sublinear increase with increasing sheet charge density.
Finally, the calculated energy shift can be connected with the experimental excitation power density, through the following rate equation
G is the generation rate of the photocarrier and is proportional to the excitation power, Δn is the photogenerated excess carrier density and Β is the bimolecular radiative recombination coefficient. Here, we ignore nonradiative recombination since the linearity of the PL intensity with the excitation power ensures the radiative dominant regime [18]. Combining Equation 6 with the numerically calculated carrier density dependence of the PL energy shift shown in Figure 3b, the following power law for the blueshift is derived:
with the power factor m’ depending on the excitation power. We show again the experimental PL peak shift in the inset of Figure 3b, along with the new power law. Transition from the low excitation regime (m’ = 1/2) to the high excitation regime (m’ = 1/4) is obvious. Between the two extremes, we can see the conventionally applied m’ = 1/3 power law regime.
Conclusions
We have analyzed the blueshift of the PL peak in a typeII QW. A oneband calculation shows that the blueshift is mainly caused by the energy shift of the confined carrier in the well. More quantitative analysis based on a selfconsistent calculation including excitonic effects illustrated the transition from a linear to a sublinear increase in the blueshift with increasing sheet charge density. Combining the calculated result with the carrier rate equation, the blueshift was found to be proportional to the mth root of the excitation power density, in which m = 1/2 ~ 1/4 and is dependent on the excitation power. The more comprehensive theory presented here predicts the 1/3power law in the literature over a limited range of carrier density only. The above power law is consistent with the experimental results obtained from a typeII GaAsSb/GaAs QW.
Abbreviations
 MOMBE:

Metalorganic molecular beam epitaxy
 PL:

Photoluminescence
 QW:

Quantum well
 XRD:

Xray diffraction.
References
Ledentsov NN, Böhrer J, Heinrichsdorff F, Grundmann M, Bimberg D, Ivanov SV, Meltser BY, Shaposhnikov SV, Yassievich IN, Faleev NN, Kop'ev PS, Alferov ZI: Radiative states in typeII GaSb/GaAs quantum wells. Phys. Rev. B 1995, 52: 14058. 10.1103/PhysRevB.52.14058
Hatami F, Grundmann M, Ledentsov NN, Heinrichsdorff F, Heitz R, Böhrer J, Bimberg D, Ruvimov SS, Werner P, Ustinov VM, Kop'ev PS, Alferov ZI: Carrier dynamics in typeII GaSb/GaAs quantum dots. Phys. Rev. B 1998, 57: 4635. 10.1103/PhysRevB.57.4635
Ribeiro E, Govorov AO, Carvalho W, MedeirosRibeiro G: AharanovoBohm signature for neutral polarized excitons in typeII quantum dot ensembles. Phys. Rev. Lett. 2004, 92: 126402.
Madureira JR, de Godoy MPF, Brasil MJSP, Iikawa F: Spatially indirect excitons in typeII quantum dots. Appl. Phys. Lett. 2007, 90: 212105. 10.1063/1.2741601
AlonsoÁlvarez D, Alén B, García JM, Ripalda JM: Optical investigation of type II GaSb/GaAs selfassembled quantum dots. Appl. Phys. Lett. 2007, 91: 263103. 10.1063/1.2827582
Kawazu T, Mano T, Noda T, Sakaki H: Optical properties of GaSb/GaAs typeII quantum dots grown by droplet epitaxy. Appl. Phys. Lett. 2009, 94: 081911. 10.1063/1.3090033
Tatebayashi J, Khoshakhlagh A, Huang SH, Dawson LR, Balakrishnan G, Huffaker DL: Formation and optical characteristics of strainrelieved and densely stacked GaSb/GaAs quantum dots. Appl. Phys. Lett. 2006, 89: 203116. 10.1063/1.2390654
Dheeraj DL, Patriarche G, Zhou H, Hoang TB, Moses AF, Grønsberg S, Helvoort AT, Fimland BO, Weman H: Growth and characterization of wurtzite GaAs nanowires with defectfree zinc blende GaasSb inserts. Nano Lett. 2008, 8: 4459. 10.1021/nl802406d
Akopian N, Patriarche G, Liu L, Harmand JC, Zwiller V: Crystal phase quantum dots. Nano Lett. 2010, 10: 1198. 10.1021/nl903534n
Muto S: On a possiblity of wavelengthdomainmultiplication memory using quantum boxes. Jpn. J. Appl. Phys. 1995, 34: L210. 10.1143/JJAP.34.L210
Geller M, Kapteyn C, MullerKirsch L, Heitz R, Bimberg D: Hole storage in GaSb/GaAs quantum dots for memory devices. Phys. Stat. Sol. (b) 2003, 238: 258. 10.1002/pssb.200303023
Suzuki K, Hogg RA, Arakawa Y: Structural and optical properties of type II GaSb/GaAs selfassembled quantum dots grown by molecular beam epitaxy. J. Appl. Phys. 1999, 85: 8349. 10.1063/1.370622
Ichii A, Tsou Y, Garmire E: An empirical rule for band offsets between IIIV alloy compounds. J. Appl. Phys. 1993, 74: 2112. 10.1063/1.354734
Noh MS, Ryou JH, Dupuis RD, Chang YL, Weissman RH: Band lineup of pseudomorphic GaAs1xSbx quantumwell structures with GaAs, GaAsP, and InGaP barriers grown by metal organic chemical vapor deposition. J. Appl. Phys. 2006, 100: 093703. 10.1063/1.2363237
Yu PY, Cardona M: Fundamentals of Semiconductors. 3rd edition. Berlin: Springer; 2005.
Vurgaftman I, Meyer JR, RamMohan LR: Band parameters for IIIV compound semiconductors and their alloys. J Appl Phys 2001, 89: 5815. 10.1063/1.1368156
Penn C, Schaffler F, Bauer G, Glutsch S: Application of numerical excitonwavefunction calculations to the question of band alignment in Si/SiGe quantum wells. Phys Rev B 1999, 59: 13314. 10.1103/PhysRevB.59.13314
Fukatsu S, Usami N, Shiraki Y: Luminescence from Si1xGex/Si quantum wells grown by Si molecularbeam epitaxy. J Vac Sci Technol B 1993, 11: 895. 10.1116/1.586732
Acknowledgements
This work was supported in part by Hokkaido University and Hokkaido Innovation through Nano Technology Support (HINTS).
Author information
Affiliations
Corresponding author
Additional information
Competing interests
The authors declare that they have no competing interests.
Authors' contributions
MJ and MS conceived and designed the experiments. MS and SM performed the sample growth. MS conducted the optical measurements. MJ carried out the numerical calculation and drafted the manuscript. HS and HK participated in the coordination of the study. IS supervised the project. All authors discussed the results and commented on the manuscript.
Authors’ original submitted files for images
Below are the links to the authors’ original submitted files for images.
Rights and permissions
Open Access This article is distributed under the terms of the Creative Commons Attribution 2.0 International License (https://creativecommons.org/licenses/by/2.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
About this article
Cite this article
Jo, M., Sato, M., Miyamura, S. et al. Origin of the blueshift of photoluminescence in a typeII heterostructure. Nanoscale Res Lett 7, 654 (2012). https://doi.org/10.1186/1556276X7654
Received:
Accepted:
Published:
DOI: https://doi.org/10.1186/1556276X7654
Keywords
 Quantum well
 typeII
 Blueshift
 Excitons
 GaSb
 GaAs
 Photoluminescence
 71.35.y: Excitons
 78.55.Cr: Photoluminescence of IIIV semiconductor
 81.15.Hi: Molecular beam epitaxy